Nonequilibrium structural states in nickel after large plastic deformation after a large plastic...
Embed Size (px)
Transcript of Nonequilibrium structural states in nickel after large plastic deformation after a large plastic...
Letters on Materials 4(2), 2014 pp. 100-103 www.lettersonmaterials.com
PACS 81.07.Bc, 61.72.Cc
Nonequilibrium structural states in nickel after large plastic deformation
I. A. Ditenberg1,2†, Е. А. Korznikova3‡, А. N. Tyumentsev1,2,4, D. Setman5, M. Kerber5, M. J. Zehetbauer5
†firstname.lastname@example.org, ‡email@example.com 1The Institute of Strength Physics and Materials Science of the Siberian Branch of RAS, Akademicheskii pr. 2 / 4,
634021, Tomsk, Russia 2The Siberian Physical-Technical Institute, Novosobornaya pl. 1, 634050, Tomsk, Russia
3The Institute of Metals Superplasticity Problems RAS, Khalturin st. 39, 450001, Ufa, Russia 4Tomsk State University, Lenin pr. 36, 634050, Tomsk, Russia
5Research Group Physics of Nanostructured Materials, Faculty of Physics, University of Vienna, Boltzmanngasse 5, A-1090, Wien, Austria
Using the methods of structural characterization and measuring the parameters of thermophysical properties, we have studied the features of highly nonequilibrium structural states that form in pure nickel in the course of high pressure torsion in Bridgman’s anvils. Keywords: high pressure torsion, nickel, microstructure, high-defect states, point defects.
By the present time perceptions have been formed that among the basic factors that are responsible for formation of a set of unusual physical and mechanical properties in submicrocrystalline and nanostructural materials, of key importance are the features of their highly nonequilibrium structure. Of special significance here are defect substructures of grain boundaries that are distinguished by high defect density, structural and thermodynamic nonequilibrium, the presence of considerable fields of local internal stresses, a change of the atomic density in near-boundary zones, etc. [1–4, etc.]. Unfortunately, in spite of a large amount of experimental data, detailed characterization of such structural states is performed only in isolated works. In particular, it has been demonstrated in the works [4–10] that an important characteristic of highly defect states in metallic materials are substructures with high values of the crystal lattice curvature, whose permanent «companions» are grain boundaries with variable misorientation vectors (∂θ/∂r≈χij) or pile-ups of continuously distributed partial disclinations. It is assumed that such states can be characterized by a high density of point defects.
In the present work a study has been conducted on the features of highly nonequilibrium structural states that are formed in pure nickel in the course of plastic deformation via high pressure torsion in Bridgman’s anvils.
2. Experimental material and procedures
The initial nickel samples of high (99.998 %) purity in the shape of disks with a diameter of 8 mm and thickness h=0.8 mm (after deformation hк≈0.6 mm) were in a structural
state with a mean grain size of around 6 μm. The samples were subjected to deformation by torsion under the pressure P≈4 GPа at room temperature to various strains determined by the number of disk revolutions (N) = 0.1, 0.5, 1, 2 and 5.
The features of thermophysical processes of bulk samples were studied using the method of differential scanning calorimetry (DSC) on a Perkin Elmer DSC7 device. Defect density was determined from the residual electrical resistivity of the deformed samples after isochronal annealings. The studies were performed in the temperature range from 50 °C to 350 °C, with a step of 25 °C and duration of annealings at each step 10 min.
Electron-microscopy study of thin foils prepared from sections parallel and perpendicular to the anvil plane was conducted on a Philips СМ-30 TWIN electron microscope at an accelerating voltage of 300 kV. Foils in the section parallel to the anvil plane were prepared by electropolishing in the solution 90 % C4H9OH + 10 % HClO4 on a Struers Tenupol device at a voltage of 35–40 V. To obtain thin foils in the sections normal to the anvil plane, a copper layer with a thickness of ≈3 mm was electrodeposited on samples with a size of 5x2x0.15 mm. Flat samples in the above-indicated sections were cut on an electrospark discharge machine and mechanically ground to the thickness ≈100 μm. Further thinning was achieved by way of argon ion sputtering at an accelerating voltage of 5 kV.
Study of the features of the defect structure of grain bulk and grain boundaries was conducted using the techniques of dark-field analysis of high continuous and discrete misorien- tations [4–9] which allow to define quantitatively the typical sizes of grain-subgrain structure and the parameters of crys- tal lattice curvature.
Ditenberg et al. /Letters on Materials 4(2), 2014 pp.100-103
3. Results Figure 1 presents an example of a calorimetric curve for heating of a sample strained at N = 2. As can be seen, two exothermic peaks in the temperature ranges 100–180 °С and 200–320 °С are observed. The peak at 120 °С corresponds to an insignificant heat generation. As established earlier , in the course of quenching experiments in this tem- perature range in pure nickel annealing of vacancies takes place, hence this peak will be subsequently referred to as the vacancy peak.
At temperatures above 180 °С a sharp decline in heat flow (fig.1) is observed, which is related to initiation of structural transformations via annihilation of dislocations and activation of recrystallization processes. The maximum values of generated heat are characterized by a peak at the temperature ≈ 220 °С.
In the temperature range 250–300 °С the peak becomes more flat, which is indicative of a less intensive heat genera- tion. Thus in the given temperature range thermally-activat- ed structural transformations evidently become completed. Exotermic peak at 358 °С corresponds to the Curie point.
During further temperature increase no significant heat effects were discovered.
It is typical for samples after large and small plastic strains that the change in residual electrical resistivity has the shape of a common S-curve, as shown in fig.2 a. With a view to separate the contributions of vacancies and dislocations, we have differentiated (dp / dt) the dependence of residual elec- trical resistivity on annealing temperature Dρ (Tann) (fig.2b).
On the produced curve (fig.2b) in the case of small strains (γ = 2.3) 2 peaks are observed. The peak at 125 °С corre-С corre- corre- sponds to the temperature of the vacancy peak on the DSC curve (fig.1). Based on this, it is assumed that the modulat- ed decrease of electrical resistivity in the temperature range 100–150 °C correlates with annealing of mono- and bivacan- cies (γ = 2.3, fig.2b). The temperature of the second peak is close to the temperature of dislocations annealing. As strain increases (γ = 47.6, fig.2b), an increase in stored energy of defects and growth of the moving force of recrystallization facilitate displacement of the dislocation peak towards low temperatures and, in fact, its merging with the vacancy peak. The sharp decline in the temperature range 150–200 °C cor- responds to annealing of dislocations.
The results of DSC and the data from measurement of residual electrical resistivity indicate completion of structural transformations at the temperature ≈300 °C.
The results of investigation into the thermophysical properties of nickel in a wider range of strains is presented in the paper .
The above-indicated features of structural changes can be visibly illustrated by micrographs showing the structural states of strained nickel after the corresponding heat treatments (fig.3).
After annealing at 125 °С the microstructure (fig.3a) practically does not differ from the microstructure which is observed immediately after straining . It has been estab- lished that a structural transformation begins at a temperature above 175 °С. After 225 °С the features of the microstructure indicate activation of the initial recrystallization processes (fig.3b) which are actually completed at 250 °С (fig.3c). At a temperature of 250 °С an intensive progress of the processes of accumulative recrystallization is observed, as a result of which the microstructure is represented by practically defect- free grains of micron (4–7 μm) sizes (fig.3d).
It follows from the above-presented results and the data from the works [7, 13] that the structural states immediately after a large plastic deformation and prior to the
Fig. 1. Dependence of heat flow on heating temperature of Ni strained at N = 2 (γ =47.6) .
Fig. 2. Examples of dependencies of specific electrical resistance on annealing temperature (a) and the temperature gradient of electrical resistivity (b) of strained Ni.
Ditenberg et al. /Letters on Materials 4(2), 2014 pp.100-103
temperature of start of active relaxation processes are highly defect (highly nonequilibrium) states.
It was established earlier [7, 13–15], during study of microstuctural and defect structure features in nickel subjected to large plastic deformation, that for such structural states it was typical to have substructures with high
values of the crystal lattice curvature and a high density of boundaries with variable misorientation vectors.
In particular, inside submicrograins nano-twins and nano-bands of reorientation were found. An example of dark-field images of the latter is shown in fig.4.